 inset of Fig. \[fig:result\](a)) into Eqs. (\[eq:scaling\]) and (\[eq:scaling-gel\]), respectively. (Further details are given in Sec. S6 of Supplemental Material.) This procedure demonstrates that we can determine $\Pi_\mathrm{mix}$ for any polymer gel by measuring a non-universal parameter $M{c^{*}}^{1/3\nu-1}$.\
*Concluding remarks*. — We have experimentally measured the osmotic pressure of polymer gels throughout the gelation process. We find that the universal EOS (\[eq:EOS\]) of the osmotic pressure for *linear*-polymer solutions describes the osmotic pressure throughout the gelation process involving both the sol and gel states (Fig. \[fig:EOS\]). In the sol states, both $\hat{\Pi}$ and $\hat{c}$ continuously increase according to the universal EOS (\[eq:EOS\]) with an increase in the average molar mass (orange filled circles in Fig. \[fig:EOS\]). In the gel states, the osmotic pressure of polymer gels is universally governed by the semidilute scaling law (\[eq:scaling-gel\]) (red star in Fig. \[fig:EOS\] and Fig. 4(b)). Here, both $\hat{\Pi}$ and $\hat{c}$ diverge to infinity, because the gel states correspond to the average molar mass $M\to\infty$ and the overlap concentration $c^{*}\to 0$. In addition, we have demonstrated that Eq. (\[eq:scaling-gel\]) enables the determination of $\Pi_\mathrm{mix}$ for any polymer gel by measuring a non-universal parameter $M{c^{*}}^{1/3\nu-1}$.

Because polymer gels are open systems that can swell and deswell by exchanging solvents with the human body, an understanding of the osmotic pressure is essential for controlling the swelling of polymer gels. Our findings are not only conceptually important to polymer physics, but also practically useful, encouraging biomedical applications of polymer gels such as soft contact lenses, adhesion barriers, sealants, and artificial vitreous humor.

We thank Masao Doi, Yuichi Masubuchi, Takashi Uneyama, and Xiang Li for their useful comments. This work was supported by the Japan Society for the Promotion of Science (JSPS) through the Grants-in-Aid for Early Career Scientists
inset of Fig.   \[fig: result\](a) ) into Eqs.   (\[eq: scaling\ ]) and (\[eq: scaling - gel\ ]), respectively. (Further details are given in Sec.   S6 of Supplemental Material .) This procedure attest that we can settle $ \Pi_\mathrm{mix}$ for any polymer gel by measuring a non - universal argument $ M{c^{*}}^{1/3\nu-1}$.\ 
 * Concluding remarks *. — We have experimentally measured the osmotic pressure of polymer gel throughout the gelation process. We find that the cosmopolitan EOS   (\[eq: EOS\ ]) of the osmotic atmospheric pressure for * linear*-polymer solutions identify the osmotic pressure throughout the gelation process involve both the sol and gel country (Fig.   \[fig: EOS\ ]). In the sol states, both $ \hat{\Pi}$ and $ \hat{c}$ continuously increase according to the universal EOS   (\[eq: EOS\ ]) with an increase in the modal molar mass (orange filled circles in Fig.   \[fig: EOS\ ]). In the gelatin states, the osmotic pressure of polymer gel is universally governed by the semidilute scaling jurisprudence   (\[eq: scaling - gel\ ]) (red star in Fig.   \[fig: EOS\ ] and Fig.   4(b) ). Here, both $ \hat{\Pi}$ and $ \hat{c}$ diverge to infinity, because the gel states correspond to the average molar bulk $ M\to\infty$ and the overlap concentration $ c^{*}\to 0$. In addition, we have demonstrated that Eq.   (\[eq: scaling - gel\ ]) enables the determination of $ \Pi_\mathrm{mix}$ for any polymer gel by measuring a non - universal parameter $ M{c^{*}}^{1/3\nu-1}$. 

 Because polymer gels are open systems that can swell and deswell by exchanging solvents with the human body, an agreement of the osmotic pressure is essential for master the bulge of polymer gels. Our findings are not only conceptually authoritative to polymer physics, but also practically useful, encourage biomedical applications of polymer gels such as soft contact lenses, adhesion barrier, sealants, and artificial vitreous humor. 

 We thank Masao   Doi, Yuichi   Masubuchi, Takashi   Uneyama, and Xiang   Li for their useful gossip. This work was back by the Japan Society for the Promotion of Science (JSPS) through the Grants - in - care for Early Career Scientists
 indet of Fig. \[fig:result\](a)) intu Eqs. (\[eq:scaling\]) cbd (\[eq:sraling-gsl\]), respeztively. (Further details are jiveb in Wec. S6 of Supplemental Mxterial.) Tjis procwdurt demonstrates thef we cak detsvmine $\'i_\mathrm{mix}$ for any polymar gel by measgrkny a non-universal parameter $M{c^{*}}^{1/3\nu-1}$.\
*Concltding rrmwrks*. — We have gxperpmqntamly measured the osmotic pressure kf polyker gels throighout the gelation procesd. We find that the unigersal EOS (\[ew:EOS\]) if the osmotkc pressurt yor *linear*-pklymer solutions describes the usmotnc pressure tyrokchout the gxlatiog process inyplving both tne sol and gel stetes (Fig. \[fig:EOS\]). In the sol states, both $\hat{\Pi}$ and $\hat{c}$ ckntinuously increqsw accmrditg tu thd uhiteraal EOD (\[eq:XOS\]) with an increase ib the average molar mwws (orange filmed ciwcjes in Fig. \[fig:EOS\]). In the gel states, the msmktic pressure of polymee gels is universally governed by the semidilute scaling law (\[eq:scaling-gel\]) (red stdr in Wig. \[yln:EOS\] qnf Fig. 4(b)). Here, both $\hat{\Pi}$ and $\hat{c}$ diverge to insjnotj, because the gel states cortedppgd to the avetage molar mass $M\to\infty$ and the ovgrlap xoncentrauion $v^{*}\to 0$. In addition, we have denonstrated tkat Eq. (\[eq:scaling-gel\]) encbles the decerminstion of $\Pi_\mathrm{mix}$ for any polgmer gel by measurinf a non-universal oarsmater $M{c^{*}}^{1/3\nu-1}$.

Because polymer gqls are o'en svstems tfat van swqll and dedwell by exchanging solvfnts cith dhe human hody, an understanding of the osmotic pressure iv evsential for gontrolling the swelling of pplymer yels. Ojr findinga are nmt only conseptually impmttant to polyker physycs, vut qlso prxztically usefuk, encouraynng biomeeical applications of lolymer gels suek qs soft contact levsef, wdiesiog barriers, sedlangs, xmd argificial vibreuus numor.

We thank Masao Dmi, Yhichi Masubuchi, Takssmi Uneyama, and Xiagg Li for theit useful comments. Uhis wmrk was xupkorted by the Japan Society for the Promltijn of Sciencq (JSIS) trrough the Grants-in-Aid for Early Career Scientistw
inset of Fig. \[fig:result\](a)) into Eqs. (\[eq:scaling\]) respectively. details are in Sec. S6 demonstrates we can determine for any polymer by measuring a non-universal parameter $M{c^{*}}^{1/3\nu-1}$.\ remarks*. — We have experimentally measured the osmotic pressure of polymer gels throughout gelation process. We find that the universal EOS (\[eq:EOS\]) of the osmotic pressure *linear*-polymer describes osmotic throughout the gelation process involving both the sol and gel states (Fig. \[fig:EOS\]). In the sol both $\hat{\Pi}$ and $\hat{c}$ continuously increase according to universal EOS (\[eq:EOS\]) with increase in the average molar (orange circles in \[fig:EOS\]). the states, the osmotic of polymer gels is universally governed by the semidilute scaling law (\[eq:scaling-gel\]) (red star in Fig. \[fig:EOS\] Fig. 4(b)). $\hat{\Pi}$ and diverge infinity, the gel states the average molar mass $M\to\infty$ and $c^{*}\to 0$. In addition, we have demonstrated that (\[eq:scaling-gel\]) enables determination of $\Pi_\mathrm{mix}$ for any polymer by measuring a non-universal parameter $M{c^{*}}^{1/3\nu-1}$. Because polymer are open systems that can swell and deswell by exchanging solvents with the human body, of the osmotic pressure essential for controlling swelling polymer Our are not conceptually important to polymer physics, but also practically useful, encouraging biomedical of polymer gels such as soft contact lenses, adhesion barriers, artificial humor. We thank Doi, Yuichi Masubuchi, Takashi and Li for their useful work supported Society the of Science (JSPS) through Grants-in-Aid for Early Career Scientists
 inset of Fig. \[fig:result\](a)) into EQs. (\[eq:scalinG\]) and (\[eQ:scAliNg-Gel\]), rEspeCtively. (Further DEtaiLs are given in Sec. S6 of SuppLemenTaL mateRIaL.) This ProceduRE dEMOnsTrAtEs tHaT We Can deTerMine $\Pi_\mAthrm{mix}$ foR anY pOlymer gel by mEAsUring a non-uNivErsal parametEr $M{C^{*}}^{1/3\nu-1}$.\
*ConClUdiNG remaRks*. — we havE experIMentalLy measureD tHE osmotIC pressuRE Of PolyMer gels throughout THe GElation process. we find ThAT tHE UniVerSal EOS (\[eq:EOs\]) oF the oSMotic prESsURE For *LInear*-polymer sOlutions desCRibEs the oSmOtiC PressuRe thrOuGHouT the gelatioN proCess involVing boTH the sol ANd gel stAtes (FiG. \[fiG:EOs\]). In tHE sOl StaTeS, BotH $\HaT{\Pi}$ ANd $\hAt{c}$ contiNuOuSly inCreaSE ACCordIng To thE univErsal EOS (\[eq:EOS\]) WitH an iNCreAse in The avEragE mOlar mAss (oraNge fiLlEd circles in Fig. \[fIg:EOs\]). In the gel StaTeS, thE oSmotiC PressuRe oF poLymer geLs is uniVErsAlLY GOvErned by the semidiluTe SCAlIng law (\[eq:ScalinG-GeL\]) (rED star in FIg. \[Fig:eOS\] aND fig. 4(b)). HEre, bOTh $\Hat{\Pi}$ and $\Hat{c}$ diVErGe To infinItY, becauSe The Gel StateS CorrEspond To the aveRage mOLar mass $M\to\inftY$ And the overlap COnCENtRAtioN $c^{*}\tO 0$. In addition, We haVE demOnstRAtEd tHAt Eq. (\[eQ:scalInG-GeL\]) Enables the determinaTiOn of $\Pi_\MathrM{mix}$ for any polYmer gel by mEASUring a noN-uniVErSAl parameter $M{c^{*}}^{1/3\nU-1}$.

BecaUse polymer GEls are opEn sysTems that Can swell aND Deswell bY exChaNgiNg sOLVeNts with the humAN Body, An UnderstAndIng of thE osMotIc pResSuRe is essenTial for cOnTrOlLiNg tHe sweLLing of poLyMer GeLs. OUr finDIngs arE not oNly cOnCePTuaLly impoRTaNT To poLyMeR phySicS, bUt alsO praCTicAlly useFul, encourAgiNG bioMeDiCal applIcations of polYmEr gels such As SofT contaCT Lenses, adHesion barriers, sealants, aND artifiCiaL vitrEous Humor.

We thAnk masao DOi, YUIchi MaSubuchI, TakaShI UnEYAma, anD xIaNg LI fOr their useFUL coMmentS. THis wOrk was sUpported by the Japan sOciEty for the PromOtiOn of sCIeNce (jsPs) ThrOuGH thE gRants-in-Aid for EaRly Career SCiENtIsts
 inset of Fig. \[fig:resul t\](a)) in to Eq s.(\[ eq :sca ling \]) and (\[eq: s cali ng-gel\]), respectivel y. (F ur t herd et ailsare giv e ni n  Se c.  S 6 o fS up pleme nta l Mater ial.) This  pr oc edure demons t ra tes that w e c an determine  $\ Pi_\ma th rm{ m ix}$for  anypolyme r  gel b y measuri ng a non- u niversa l pa rame ter $M{c^{*}}^{1/ 3 \n u -1}$.\
*Conclu ding r em a rk s * . —  We  have expe ri menta l ly meas u re d t heo smotic pressu re of polym e r g els th ro ugh o ut the  gela ti o n p rocess. Wefind  that the  unive r sal EOS (\[eq:E OS\])ofthe  osm o ti cpre ss u ref or  *l i nea r*-polym er  s oluti onsd e s c ribe s t he o smoti c pressure th rou ghou t  th e gel ation  pro ce ss in volvin g bot hthe sol and gel  sta tes (Fig.  \[ fi g:E OS \]).I n thesol  st ates, b oth $\h a t{\ Pi } $ an d $\hat{c}$ contin uo u s ly  increas e acco r di ng to the u ni ver salE O S (\[ eq:E O S\ ]) withan inc r ea se  in the  a verage  m ola r m ass ( o rang e fill ed circl es in Fig. \[fig:EOS \ ]). In the ge l  s t a te s , th e o smotic pres sure of p olym e rgel s  is u niver sa l ly governed by the sem id ilutescali ng law (\[eq: scaling-ge l \ ] ) (red s tari nF ig. \[fig:EOS\ ] and  Fig. 4(b) ) . Here,both$\hat{\P i}$ and $ \ h at{c}$ d ive rge  to  in f i ni ty, because t h e  gel  s tates c orr espondtothe  av era ge  molar ma ss $M\to \i nf ty $and  theo verlap c on cen tr ati on $c ^ {*}\to  0$.In a dd it i on,  we hav e  d e m onst ra te d th atEq . (\[ eq:s c ali ng-gel\ ]) enable s t h e de te rm ination  of $\Pi_\mat hr m{mix}$ fo rany  polym e r  gel bymeasuring a non-univers a l param ete r $M{ c^{* }}^{1/3\n u-1 }$.

B eca u se pol ymer g els a re  op e n  syst e m stha tcan swella n d d eswel lby e xchangi ng solvents with t h e h uman body, an  un ders t a nd ing of the  o s mot i c  pressure is es sential fo rc on trolling t h e s we lling o f polym er ge l s. Ourfindingsare not o nl y co n c ept ually impo rtant to  polymerp hysic s ,but a lso  pract ic all y use ful, e n cou ragin g biom ed ical a pplic at ions ofpolymer gels such as so ft con tactlen ses, adhe sio n  ba rriers, s eala nts, and a rti fic ial v itr e ous h umor . 
Wet hankMasa o  Doi, Yui c hi  Ma s u bu chi, Takash i U ney ama,and XiangLi f or their useful c o mments. This w orkw a s s upp o rted  b y the Japan So cie ty f or the P ro motion of S cience ( JS P S) th roughthe Gr ants-in - A id for Ea rlyCar eer Scien tis ts 
 inset_of Fig. \[fig:result\](a))_into Eqs. (\[eq:scaling\]) and (\[eq:scaling-gel\]),_respectively. (Further_details_are given_in_Sec. S6 of Supplemental_Material.) This procedure_demonstrates that we can_determine $\Pi_\mathrm{mix}$ for_any_polymer gel by measuring a non-universal parameter $M{c^{*}}^{1/3\nu-1}$.\
*Concluding remarks*. — We have experimentally measured_the_osmotic pressure_of_polymer_gels throughout the gelation process._We find that the universal_EOS (\[eq:EOS\]) of_the osmotic pressure for *linear*-polymer solutions describes the_osmotic_pressure throughout the_gelation process involving both the sol and gel states_(Fig. \[fig:EOS\]). In the sol states, both_$\hat{\Pi}$ and $\hat{c}$_continuously_increase_according to the universal_EOS (\[eq:EOS\]) with an increase in the_average molar mass (orange filled circles_in Fig. \[fig:EOS\]). In the gel states, the_osmotic pressure of polymer gels is_universally governed by the semidilute_scaling law (\[eq:scaling-gel\])_(red star in Fig. \[fig:EOS\] and_Fig. 4(b)). Here, both_$\hat{\Pi}$ and_$\hat{c}$ diverge to_infinity, because the gel states correspond_to the average_molar mass $M\to\infty$ and the overlap_concentration_$c^{*}\to 0$. In_addition,_we_have demonstrated_that Eq. (\[eq:scaling-gel\]) enables_the_determination of_$\Pi_\mathrm{mix}$_for any polymer gel by measuring_a_non-universal parameter $M{c^{*}}^{1/3\nu-1}$.

Because polymer gels are open_systems that can swell_and_deswell by exchanging solvents_with the human body, an_understanding of the osmotic pressure is_essential for_controlling the_swelling of polymer gels. Our findings are not only conceptually important_to polymer physics, but also practically_useful, encouraging biomedical applications_of polymer_gels_such as soft_contact_lenses, adhesion_barriers, sealants, and artificial vitreous humor.

We thank_Masao Doi, Yuichi Masubuchi,_Takashi Uneyama, and Xiang Li for their useful_comments. This work was_supported_by the Japan Society for the_Promotion of Science (JSPS) through the_Grants-in-Aid for Early Career Scientists